data_njy1
_audit_creation_date              2015-11-10
_audit_creation_method
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_publ_contact_author_address      ?
_publ_contact_author_email        ?
_publ_contact_author_name         ''
_publ_contact_author_phone        ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2008). Acta Cryst. A64, 112-122.

Sheldrick, G.M. (2015). Acta Cryst. C71, 3-8.
;
_chemical_name_common             ?
_chemical_name_systematic
;
 ? 
;
_chemical_formula_moiety          '0.33(Cs30 Mn3 Na9 Nb27 O387 Si9 W81), 9(O)'
_chemical_formula_sum             'Cs10 H42 Mn Na3 Nb9 O138 Si3 W27'
_chemical_formula_weight          9587.75
_chemical_absolute_configuration  ?
_chemical_melting_point           ?
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'Cs' 'Cs' -0.3680 2.1192
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn' 'Mn' 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Nb' 'Nb' -2.0727 0.6215
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si' 'Si' 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'W' 'W' -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H' 'H' 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na' 'Na' 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system       'trigonal'
_space_group_IT_number            160
_space_group_name_H-M_alt         'R 3 m'
_space_group_name_Hall            'R 3 -2"'
loop_
  _space_group_symop_operation_xyz
 'x, y, z'
 '-y, x-y, z'
 '-x+y, -x, z'
 '-y, -x, z'
 'x, x-y, z'
 '-x+y, y, z'
 'x+2/3, y+1/3, z+1/3'
 '-y+2/3, x-y+1/3, z+1/3'
 '-x+y+2/3, -x+1/3, z+1/3'
 '-y+2/3, -x+1/3, z+1/3'
 'x+2/3, x-y+1/3, z+1/3'
 '-x+y+2/3, y+1/3, z+1/3'
 'x+1/3, y+2/3, z+2/3'
 '-y+1/3, x-y+2/3, z+2/3'
 '-x+y+1/3, -x+2/3, z+2/3'
 '-y+1/3, -x+2/3, z+2/3'
 'x+1/3, x-y+2/3, z+2/3'
 '-x+y+1/3, y+2/3, z+2/3'

_cell_length_a                    30.722(2)
_cell_length_b                    30.722
_cell_length_c                    16.0353(12)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 120
_cell_volume                      13107(2)
_cell_formula_units_Z             3
_cell_measurement_reflns_used     4202
_cell_measurement_temperature     293(2)
_cell_measurement_theta_max       24.609
_cell_measurement_theta_min       2.30
_shelx_estimated_absorpt_T_max    0.149
_shelx_estimated_absorpt_T_min    0.105
_exptl_absorpt_coefficient_mu     20.494
_exptl_absorpt_correction_T_max   0.7457
_exptl_absorpt_correction_T_min   0.3343
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_process_details
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.1764 before and 0.0575 after correction.
The Ratio of minimum to maximum transmission is 0.4483.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details    ?
_exptl_crystal_colour             purple
_exptl_crystal_density_diffrn     3.644
_exptl_crystal_density_meas       .
_exptl_crystal_density_method     'not measured'
_exptl_crystal_description        block
_exptl_crystal_F_000              12489
_exptl_crystal_size_max           0.2
_exptl_crystal_size_mid           0.15
_exptl_crystal_size_min           0.15
_exptl_special_details
;
 ? 
;
_exptl_transmission_factor_max    ?
_exptl_transmission_factor_min    ?
_diffrn_reflns_av_R_equivalents   0.0677
_diffrn_reflns_av_unetI/netI      0.0605
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max        25
_diffrn_reflns_limit_h_min        -36
_diffrn_reflns_limit_k_max        36
_diffrn_reflns_limit_k_min        -36
_diffrn_reflns_limit_l_max        19
_diffrn_reflns_limit_l_min        -18
_diffrn_reflns_number             22609
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full         25.099
_diffrn_reflns_theta_max          25.099
_diffrn_reflns_theta_min          2.296
_diffrn_ambient_temperature       293(2)
_diffrn_detector_area_resol_mean  ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type   'Bruker APEX-II CCD'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_radiation_monochromator   'graphite'
_diffrn_radiation_type            MoK\a
_diffrn_radiation_wavelength      0.71073
_diffrn_source                    ?
_diffrn_standards_number          0
_reflns_Friedel_coverage          0.994
_reflns_Friedel_fraction_full     0.996
_reflns_Friedel_fraction_max      0.996
_reflns_number_gt                 4357
_reflns_number_total              5265
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression      'I > 2σ(I)'
_computing_cell_refinement        'Bruker SAINT'
_computing_data_collection        'Bruker APEX2'
_computing_data_reduction         'Bruker SAINT'
_computing_molecular_graphics     'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material   'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement   'ShelXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution     'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max          2.313
_refine_diff_density_min          -1.352
_refine_diff_density_rms          0.304
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack    0.669(18)
_refine_ls_extinction_coef        .
_refine_ls_extinction_method      none
_refine_ls_goodness_of_fit_ref    1.012
_refine_ls_hydrogen_treatment     undef
_refine_ls_matrix_type            full
_refine_ls_number_parameters      200
_refine_ls_number_reflns          5265
_refine_ls_number_restraints      7
_refine_ls_R_factor_all           0.0612
_refine_ls_R_factor_gt            0.0419
_refine_ls_restrained_S_all       1.012
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0654P)²+124.8428P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme       calc
_refine_ls_wR_factor_gt           0.1025
_refine_ls_wR_factor_ref          0.1129
_refine_special_details
;
 Refined as a 2-component inversion twin.
;
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.331(18) 0.669(18)
2. Uiso/Uaniso restraints and constraints
Uanis(Na1) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
;
_atom_sites_solution_hydrogens    .
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_site_symmetry_order
  _atom_site_calc_flag
  _atom_site_refinement_flags_posn
  _atom_site_refinement_flags_adp
  _atom_site_refinement_flags_occupancy
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 W1 W 0.44431(4) 0.10733(4) 0.22463(10) 0.0317(3) Uani 1 1 d . . . . .
 W2 W 0.44639(4) 0.16261(4) 0.04407(8) 0.0312(3) Uani 1 1 d . . . . .
 W3 W 0.33104(6) 0.16552(3) 0.10467(13) 0.0341(4) Uani 1 2 d S T P . .
 W4 W 0.32817(4) 0.10915(4) 0.28639(9) 0.0366(3) Uani 1 1 d . . . . .
 W5 W 0.43933(4) 0.27427(5) 0.42612(8) 0.0342(3) Uani 1 1 d . . . . .
 Nb1 Nb 0.54448(10) 0.27224(5) 0.3640(2) 0.0121(6) Uani 1 2 d S T P . .
 Nb2 Nb 0.54628(10) 0.21492(10) 0.16832(19) 0.0354(7) Uani 1 1 d . . . . .
 Mn1 Mn 0.6667 0.3333 0.4953(7) 0.030(2) Uani 1 6 d S T P . .
 Si1 Si 0.4391(4) 0.21957(18) 0.2299(7) 0.020(2) Uani 1 2 d S T P . .
 Cs1 Cs 0.31714(9) 0.02283(9) 0.07953(19) 0.0644(7) Uani 1 1 d . . . . .
 Cs2 Cs 0.0000 0.0000 0.9056(3) 0.0306(10) Uani 1 6 d S T P . .
 Cs3 Cs 0.17366(11) 0.08683(6) 0.0425(2) 0.0524(8) Uani 1 2 d S T P . .
 Na1 Na 0.1575(3) 0.3151(5) 0.5334(9) 0.024(3) Uani 1 2 d S TU P . .
 O1 O 0.6027(10) 0.3014(5) 0.4206(17) 0.030(6) Uiso 1 2 d S T P . .
 O2 O 0.5549(7) 0.2331(7) 0.2811(12) 0.032(5) Uiso 1 1 d . . . . .
 O3 O 0.5082(7) 0.2992(7) 0.4392(13) 0.034(5) Uiso 1 1 d . . . . .
 O4 O 0.4583(8) 0.2292(4) 0.3284(15) 0.016(5) Uiso 1 2 d S T P . .
 O5 O 0.6109(5) 0.2218(11) 0.1428(19) 0.036(7) Uiso 1 2 d S T P . .
 O6 O 0.5612(10) 0.2806(5) 0.1384(16) 0.028(6) Uiso 1 2 d S T P . .
 O7 O 0.5113(7) 0.1404(7) 0.2073(13) 0.033(5) Uiso 1 1 d . . . . .
 O8 O 0.5151(7) 0.1877(7) 0.0568(12) 0.031(4) Uiso 1 1 d . . . . .
 O9 O 0.4591(6) 0.1867(6) 0.1828(11) 0.024(4) Uiso 1 1 d . . . . .
 O10 O 0.4321(8) 0.0458(7) 0.2439(14) 0.040(5) Uiso 1 1 d . . . . .
 O11 O 0.4515(7) 0.1311(7) 0.3370(13) 0.033(4) Uiso 1 1 d . . . . .
 O12 O 0.4310(7) 0.1017(7) 0.1055(13) 0.033(5) Uiso 1 1 d . . . . .
 O13 O 0.3737(7) 0.0928(7) 0.2397(14) 0.035(5) Uiso 1 1 d . . . . .
 O14 O 0.4376(8) 0.1376(8) -0.0563(14) 0.043(5) Uiso 1 1 d . . . . .
 O15 O 0.4576(11) 0.2288(5) 0.0192(18) 0.038(7) Uiso 1 2 d S T P . .
 O16 O 0.3772(7) 0.1466(7) 0.0686(13) 0.033(5) Uiso 1 1 d . . . . .
 O17 O 0.2883(11) 0.1441(6) 0.021(2) 0.045(8) Uiso 1 2 d S T P . .
 O18 O 0.2991(8) 0.1063(8) 0.1780(13) 0.037(5) Uiso 1 1 d . . . . .
 O19 O 0.3776(10) 0.1888(5) 0.2270(18) 0.031(6) Uiso 1 2 d S T P . .
 O20 O 0.2824(8) 0.0511(8) 0.3199(14) 0.041(5) Uiso 1 1 d . . . . .
 O21 O 0.2993(11) 0.1496(6) 0.317(2) 0.045(8) Uiso 1 2 d S T P . .
 O22 O 0.4278(8) 0.3031(8) 0.5097(15) 0.047(6) Uiso 1 1 d . . . . .
 O23 O 0.4245(10) 0.2122(5) 0.4815(18) 0.036(7) Uiso 1 2 d S T P . .
 O24 O 0.3723(7) 0.2368(7) 0.3768(13) 0.037(5) Uiso 1 1 d . . . . .
 O1W O 0.6361(11) 0.272(2) 0.583(3) 0.109(17) Uiso 1 2 d S T P . .
 O2W O 0.1941(7) 0.3882(14) 0.513(2) 0.062(10) Uiso 1 2 d S T P . .
 O3W O 0.219(2) 0.1097(10) 0.703(3) 0.093(15) Uiso 1 2 d S T P . .
 O4W O 0.145(2) 0.0726(10) 0.616(4) 0.111(17) Uiso 1 2 d S T P . .
 O5W O 0.5457(10) 0.091(2) 0.087(4) 0.101(16) Uiso 1 2 d S T P . .
 O6W O 0.600(3) 0.3000(15) -0.023(5) 0.16(3) Uiso 1 2 d S T P . .
 O7W O 0.308(3) 0.1542(13) 0.520(5) 0.16(3) Uiso 1 2 d S T P . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 W1 Cs1 4.156(3) . ?
 W1 Cs1 3.956(3) 9 ?
 W1 Cs3 4.371(3) 9 ?
 W1 O7 1.803(19) . ?
 W1 O9 2.344(17) . ?
 W1 O10 1.761(19) . ?
 W1 O11 1.91(2) . ?
 W1 O12 1.94(2) . ?
 W1 O13 2.00(2) . ?
 W2 Cs1 4.181(3) . ?
 W2 O8 1.863(19) . ?
 W2 O9 2.315(18) . ?
 W2 O12 1.951(19) . ?
 W2 O14 1.74(2) . ?
 W2 O15 1.927(8) . ?
 W2 O16 1.969(19) . ?
 W3 Cs1 4.206(3) 5 ?
 W3 Cs1 4.206(3) . ?
 W3 Cs3 4.304(3) . ?
 W3 O16 1.871(19) 5 ?
 W3 O16 1.871(19) . ?
 W3 O17 1.76(3) . ?
 W3 O18 1.97(2) . ?
 W3 O18 1.97(2) 5 ?
 W3 O19 2.32(3) . ?
 W4 Cs1 4.241(3) 9 ?
 W4 Cs1 4.154(3) . ?
 W4 O13 1.86(2) . ?
 W4 O18 1.94(2) . ?
 W4 O19 2.342(19) . ?
 W4 O20 1.71(2) . ?
 W4 O21 1.920(15) . ?
 W4 O24 1.87(2) 5 ?
 W5 Cs1 3.973(3) 12 ?
 W5 Cs3 4.4748(14) 8 ?
 W5 O3 1.867(19) . ?
 W5 O4 2.351(17) . ?
 W5 O11 1.91(2) 5 ?
 W5 O22 1.74(2) . ?
 W5 O23 1.939(15) . ?
 W5 O24 1.96(2) . ?
 Nb1 Cs2 3.819(4) 7_554 ?
 Nb1 Cs3 4.115(2) 8 ?
 Nb1 Cs3 4.115(2) 9 ?
 Nb1 O1 1.80(3) . ?
 Nb1 O2 1.92(2) . ?
 Nb1 O2 1.92(2) 5 ?
 Nb1 O3 2.08(2) . ?
 Nb1 O3 2.08(2) 5 ?
 Nb1 O4 2.36(2) . ?
 Nb2 Cs2 3.840(3) 7_554 ?
 Nb2 Cs3 4.095(4) 9 ?
 Nb2 O2 1.87(2) . ?
 Nb2 O5 1.932(8) . ?
 Nb2 O6 1.894(9) . ?
 Nb2 O7 2.08(2) . ?
 Nb2 O8 2.00(2) . ?
 Nb2 O9 2.377(17) . ?
 Mn1 Cs2 4.110(12) 7_554 ?
 Mn1 O1 2.08(3) . ?
 Mn1 O1 2.08(3) 2_655 ?
 Mn1 O1 2.08(3) 3_665 ?
 Mn1 O1W 2.15(6) 2_655 ?
 Mn1 O1W 2.15(6) . ?
 Mn1 O1W 2.15(6) 3_665 ?
 Si1 O4 1.66(3) . ?
 Si1 O9 1.609(18) 5 ?
 Si1 O9 1.609(18) . ?
 Si1 O19 1.64(3) . ?
 Cs1 W1 3.956(3) 14_544 ?
 Cs1 W5 3.973(3) 18_544 ?
 Cs1 O10 3.14(2) 14_544 ?
 Cs1 O11 3.357(19) 14_544 ?
 Cs1 O12 3.131(19) . ?
 Cs1 O13 3.24(2) . ?
 Cs1 O13 3.63(2) 14_544 ?
 Cs1 O16 3.298(19) . ?
 Cs1 O18 3.29(2) . ?
 Cs1 O20 3.74(2) 14_544 ?
 Cs1 O22 3.28(2) 18_544 ?
 Cs1 O24 3.71(2) 18_544 ?
 Cs2 O2 3.340(19) 17_445 ?
 Cs2 O2 3.340(18) 14_545 ?
 Cs2 O2 3.340(19) 13_445 ?
 Cs2 O2 3.340(18) 18_545 ?
 Cs2 O2 3.340(19) 15 ?
 Cs2 O2 3.340(19) 16 ?
 Cs2 O5 3.34(3) 15 ?
 Cs2 O5 3.34(3) 14_545 ?
 Cs2 O5 3.34(3) 13_445 ?
 Cs2 O6 3.24(3) 14_545 ?
 Cs2 O6 3.24(3) 15 ?
 Cs2 O6 3.24(3) 13_445 ?
 Cs3 Nb1 4.115(2) 15_554 ?
 Cs3 Nb2 4.095(4) 16_554 ?
 Cs3 Nb2 4.095(4) 14_544 ?
 Cs3 O2 3.116(19) 16_554 ?
 Cs3 O2 3.116(19) 14_544 ?
 Cs3 O3 3.392(19) 18_544 ?
 Cs3 O3 3.392(19) 15_554 ?
 Cs3 O7 3.29(2) 14_544 ?
 Cs3 O7 3.29(2) 16_554 ?
 Cs3 O11 3.641(19) 16_554 ?
 Cs3 O11 3.641(19) 14_544 ?
 Cs3 O17 3.07(3) . ?
 Na1 O17 2.99(4) 15 ?
 Na1 O2W 1.97(4) . ?
 O1 Cs2 3.37(3) 7_554 ?
 O2 Cs2 3.340(18) 7_554 ?
 O2 Cs3 3.116(19) 9 ?
 O3 Cs3 3.392(19) 8 ?
 O4 W5 2.351(17) 5 ?
 O5 Nb2 1.932(8) 6_655 ?
 O5 Cs2 3.34(3) 7_554 ?
 O6 Nb2 1.894(9) 5 ?
 O6 Cs2 3.24(3) 7_554 ?
 O7 Cs3 3.29(2) 9 ?
 O10 Cs1 3.14(2) 9 ?
 O11 W5 1.91(2) 5 ?
 O11 Cs1 3.357(19) 9 ?
 O11 Cs3 3.640(19) 9 ?
 O13 Cs1 3.63(2) 9 ?
 O15 W2 1.927(8) 5 ?
 O17 Na1 2.99(4) 8_554 ?
 O19 W4 2.342(19) 5 ?
 O20 Cs1 3.74(2) 9 ?
 O21 W4 1.919(15) 5 ?
 O22 Cs1 3.28(2) 12 ?
 O23 W5 1.939(15) 5 ?
 O24 W4 1.87(2) 5 ?
 O24 Cs1 3.71(2) 12 ?
 O2W O5W 1.79(7) 7_455 ?
 O3W O5W 1.01(6) 14_545 ?
 O5W O2W 1.79(7) 13_544 ?
 O5W O3W 1.01(6) 9_554 ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 Cs1 W1 Cs1 88.11(5) 9 . ?
 Cs1 W1 Cs3 164.88(6) . 9 ?
 Cs1 W1 Cs3 85.96(7) 9 9 ?
 O7 W1 Cs1 126.4(6) . 9 ?
 O7 W1 Cs1 135.8(6) . . ?
 O7 W1 Cs3 43.1(6) . 9 ?
 O7 W1 O9 78.3(7) . . ?
 O7 W1 O11 92.8(8) . . ?
 O7 W1 O12 91.6(9) . . ?
 O7 W1 O13 161.7(8) . . ?
 O9 W1 Cs1 97.0(4) . . ?
 O9 W1 Cs1 134.7(4) . 9 ?
 O9 W1 Cs3 97.0(4) . 9 ?
 O10 W1 Cs1 78.3(7) . . ?
 O10 W1 Cs1 50.4(7) . 9 ?
 O10 W1 Cs3 87.2(7) . 9 ?
 O10 W1 O7 101.7(9) . . ?
 O10 W1 O9 173.4(9) . . ?
 O10 W1 O11 99.6(9) . . ?
 O10 W1 O12 98.9(9) . . ?
 O10 W1 O13 96.6(9) . . ?
 O11 W1 Cs1 131.1(6) . . ?
 O11 W1 Cs1 57.9(6) . 9 ?
 O11 W1 Cs3 55.3(6) . 9 ?
 O11 W1 O9 87.0(7) . . ?
 O11 W1 O12 159.6(8) . . ?
 O11 W1 O13 82.9(8) . . ?
 O12 W1 Cs1 132.0(6) . 9 ?
 O12 W1 Cs1 45.9(6) . . ?
 O12 W1 Cs3 134.3(6) . 9 ?
 O12 W1 O9 74.5(7) . . ?
 O12 W1 O13 86.7(8) . . ?
 O13 W1 Cs1 65.8(6) . 9 ?
 O13 W1 Cs1 49.6(6) . . ?
 O13 W1 Cs3 138.0(6) . 9 ?
 O13 W1 O9 83.8(7) . . ?
 O8 W2 Cs1 135.1(6) . . ?
 O8 W2 O9 77.7(7) . . ?
 O8 W2 O12 91.3(8) . . ?
 O8 W2 O15 91.1(10) . . ?
 O8 W2 O16 160.3(9) . . ?
 O9 W2 Cs1 96.9(4) . . ?
 O12 W2 Cs1 45.3(6) . . ?
 O12 W2 O9 75.1(7) . . ?
 O12 W2 O16 86.9(8) . . ?
 O14 W2 Cs1 79.3(7) . . ?
 O14 W2 O8 100.3(9) . . ?
 O14 W2 O9 172.3(8) . . ?
 O14 W2 O12 97.7(9) . . ?
 O14 W2 O15 100.4(11) . . ?
 O14 W2 O16 99.4(9) . . ?
 O15 W2 Cs1 133.5(8) . . ?
 O15 W2 O9 87.1(9) . . ?
 O15 W2 O12 161.0(10) . . ?
 O15 W2 O16 84.6(10) . . ?
 O16 W2 Cs1 50.5(5) . . ?
 O16 W2 O9 82.9(7) . . ?
 Cs1 W3 Cs1 165.06(8) . 5 ?
 Cs1 W3 Cs3 83.82(4) 5 . ?
 Cs1 W3 Cs3 83.82(4) . . ?
 O16 W3 Cs1 49.1(6) . . ?
 O16 W3 Cs1 135.3(6) . 5 ?
 O16 W3 Cs1 49.1(6) 5 5 ?
 O16 W3 Cs1 135.3(6) 5 . ?
 O16 W3 Cs3 124.5(6) 5 . ?
 O16 W3 Cs3 124.5(6) . . ?
 O16 W3 O16 87.1(12) . 5 ?
 O16 W3 O18 90.2(8) . . ?
 O16 W3 O18 158.9(9) . 5 ?
 O16 W3 O18 158.9(9) 5 . ?
 O16 W3 O18 90.2(8) 5 5 ?
 O16 W3 O19 84.9(8) . . ?
 O16 W3 O19 84.9(8) 5 . ?
 O17 W3 O16 100.9(10) . . ?
 O17 W3 O16 100.9(10) . 5 ?
 O17 W3 O18 100.2(10) . 5 ?
 O17 W3 O18 100.2(10) . . ?
 O17 W3 O19 172.0(13) . . ?
 O18 W3 Cs1 49.5(6) . . ?
 O18 W3 Cs1 133.5(6) 5 . ?
 O18 W3 Cs1 49.5(6) 5 5 ?
 O18 W3 Cs1 133.5(6) . 5 ?
 O18 W3 Cs3 73.6(6) 5 . ?
 O18 W3 Cs3 73.6(6) . . ?
 O18 W3 O18 84.9(12) 5 . ?
 O18 W3 O19 74.0(8) 5 . ?
 O18 W3 O19 74.0(8) . . ?
 O13 W4 Cs1 58.3(7) . 9 ?
 O13 W4 Cs1 48.7(6) . . ?
 O13 W4 O18 91.1(9) . . ?
 O13 W4 O19 86.3(8) . . ?
 O13 W4 O21 158.6(10) . . ?
 O13 W4 O24 87.0(9) . 5 ?
 O18 W4 Cs1 134.0(6) . 9 ?
 O18 W4 Cs1 50.7(6) . . ?
 O18 W4 O19 74.0(9) . . ?
 O19 W4 Cs1 98.4(6) . . ?
 O19 W4 Cs1 129.8(6) . 9 ?
 O20 W4 Cs1 79.8(7) . . ?
 O20 W4 Cs1 61.4(7) . 9 ?
 O20 W4 O13 100.4(10) . . ?
 O20 W4 O18 96.6(10) . . ?
 O20 W4 O19 168.7(9) . . ?
 O20 W4 O21 100.9(11) . . ?
 O20 W4 O24 104.3(10) . 5 ?
 O21 W4 Cs1 134.7(10) . . ?
 O21 W4 Cs1 136.1(9) . 9 ?
 O21 W4 O18 84.7(12) . . ?
 O21 W4 O19 72.3(10) . . ?
 O24 W4 Cs1 134.8(6) 5 . ?
 O24 W4 Cs1 60.9(6) 5 9 ?
 O24 W4 O18 159.0(9) 5 . ?
 O24 W4 O19 85.0(9) 5 . ?
 O24 W4 O21 89.5(11) 5 . ?
 Cs1 W5 Cs3 84.36(6) 12 8 ?
 O3 W5 Cs1 125.8(6) . 12 ?
 O3 W5 Cs3 44.1(6) . 8 ?
 O3 W5 O4 75.7(8) . . ?
 O3 W5 O11 91.1(9) . 5 ?
 O3 W5 O23 90.8(10) . . ?
 O3 W5 O24 158.6(9) . . ?
 O4 W5 Cs1 134.2(5) . 12 ?
 O4 W5 Cs3 94.1(5) . 8 ?
 O11 W5 Cs1 57.4(6) 5 12 ?
 O11 W5 Cs3 52.5(6) 5 8 ?
 O11 W5 O4 85.7(7) 5 . ?
 O11 W5 O23 158.9(10) 5 . ?
 O11 W5 O24 83.7(8) 5 . ?
 O22 W5 Cs1 54.3(8) . 12 ?
 O22 W5 Cs3 88.2(7) . 8 ?
 O22 W5 O3 100.5(9) . . ?
 O22 W5 O4 171.4(9) . . ?
 O22 W5 O11 102.3(10) . 5 ?
 O22 W5 O23 98.0(11) . . ?
 O22 W5 O24 100.8(10) . . ?
 O23 W5 Cs1 134.8(8) . 12 ?
 O23 W5 Cs3 134.6(8) . 8 ?
 O23 W5 O4 74.5(8) . . ?
 O23 W5 O24 86.9(10) . . ?
 O24 W5 Cs1 67.9(6) . 12 ?
 O24 W5 Cs3 136.2(6) . 8 ?
 O24 W5 O4 83.2(8) . . ?
 Cs2 Nb1 Cs3 80.20(5) 7_554 8 ?
 Cs2 Nb1 Cs3 80.20(5) 7_554 9 ?
 Cs3 Nb1 Cs3 153.02(10) 9 8 ?
 O1 Nb1 Cs2 62.1(9) . 7_554 ?
 O1 Nb1 Cs3 77.25(9) . 9 ?
 O1 Nb1 Cs3 77.25(9) . 8 ?
 O1 Nb1 O2 103.0(8) . 5 ?
 O1 Nb1 O2 103.0(8) . . ?
 O1 Nb1 O3 96.2(9) . . ?
 O1 Nb1 O3 96.2(9) . 5 ?
 O1 Nb1 O4 163.6(11) . . ?
 O2 Nb1 Cs2 61.0(6) . 7_554 ?
 O2 Nb1 Cs2 61.0(6) 5 7_554 ?
 O2 Nb1 Cs3 133.5(6) 5 9 ?
 O2 Nb1 Cs3 46.4(6) 5 8 ?
 O2 Nb1 Cs3 46.4(6) . 9 ?
 O2 Nb1 Cs3 133.5(6) . 8 ?
 O2 Nb1 O2 90.2(12) . 5 ?
 O2 Nb1 O3 89.8(8) 5 . ?
 O2 Nb1 O3 89.8(8) . 5 ?
 O2 Nb1 O3 160.3(8) . . ?
 O2 Nb1 O3 160.3(8) 5 5 ?
 O2 Nb1 O4 88.5(7) . . ?
 O2 Nb1 O4 88.5(7) 5 . ?
 O3 Nb1 Cs2 134.5(5) 5 7_554 ?
 O3 Nb1 Cs2 134.5(5) . 7_554 ?
 O3 Nb1 Cs3 136.8(6) . 9 ?
 O3 Nb1 Cs3 55.3(5) . 8 ?
 O3 Nb1 Cs3 136.8(6) 5 8 ?
 O3 Nb1 Cs3 55.3(5) 5 9 ?
 O3 Nb1 O3 83.8(11) . 5 ?
 O3 Nb1 O4 71.9(7) 5 . ?
 O3 Nb1 O4 71.9(7) . . ?
 O4 Nb1 Cs2 134.4(6) . 7_554 ?
 O4 Nb1 Cs3 103.48(5) . 9 ?
 O4 Nb1 Cs3 103.47(5) . 8 ?
 Cs2 Nb2 Cs3 80.22(9) 7_554 9 ?
 O2 Nb2 Cs2 60.4(6) . 7_554 ?
 O2 Nb2 Cs3 46.4(6) . 9 ?
 O2 Nb2 O5 100.8(11) . . ?
 O2 Nb2 O6 90.2(10) . . ?
 O2 Nb2 O7 87.5(8) . . ?
 O2 Nb2 O8 162.5(8) . . ?
 O2 Nb2 O9 88.9(7) . . ?
 O5 Nb2 Cs2 60.6(9) . 7_554 ?
 O5 Nb2 Cs3 76.1(9) . 9 ?
 O5 Nb2 O7 97.0(10) . . ?
 O5 Nb2 O8 96.1(10) . . ?
 O5 Nb2 O9 165.6(10) . . ?
 O6 Nb2 Cs2 57.3(8) . 7_554 ?
 O6 Nb2 Cs3 132.1(8) . 9 ?
 O6 Nb2 O5 98.1(12) . . ?
 O6 Nb2 O7 164.9(9) . . ?
 O6 Nb2 O8 91.7(9) . . ?
 O6 Nb2 O9 92.4(9) . . ?
 O7 Nb2 Cs2 132.6(5) . 7_554 ?
 O7 Nb2 Cs3 53.0(5) . 9 ?
 O7 Nb2 O9 72.6(7) . . ?
 O8 Nb2 Cs2 133.7(5) . 7_554 ?
 O8 Nb2 Cs3 136.0(5) . 9 ?
 O8 Nb2 O7 86.1(8) . . ?
 O8 Nb2 O9 73.7(7) . . ?
 O9 Nb2 Cs2 133.8(4) . 7_554 ?
 O9 Nb2 Cs3 103.9(4) . 9 ?
 O1 Mn1 Cs2 54.9(8) 2_655 7_554 ?
 O1 Mn1 Cs2 54.9(8) 3_665 7_554 ?
 O1 Mn1 Cs2 54.9(8) . 7_554 ?
 O1 Mn1 O1 90.2(11) . 3_665 ?
 O1 Mn1 O1 90.2(11) 2_655 . ?
 O1 Mn1 O1 90.2(11) 2_655 3_665 ?
 O1 Mn1 O1W 93.8(12) . . ?
 O1 Mn1 O1W 174.3(18) 2_655 3_665 ?
 O1 Mn1 O1W 93.8(12) . 3_665 ?
 O1 Mn1 O1W 93.8(12) 3_665 3_665 ?
 O1 Mn1 O1W 93.8(12) 2_655 2_655 ?
 O1 Mn1 O1W 93.8(12) 3_665 2_655 ?
 O1 Mn1 O1W 93.8(12) 2_655 . ?
 O1 Mn1 O1W 174.3(18) 3_665 . ?
 O1 Mn1 O1W 174.3(18) . 2_655 ?
 O1W Mn1 Cs2 130.9(15) 2_655 7_554 ?
 O1W Mn1 Cs2 130.9(15) . 7_554 ?
 O1W Mn1 Cs2 130.9(15) 3_665 7_554 ?
 O1W Mn1 O1W 82(2) 2_655 . ?
 O1W Mn1 O1W 82(2) . 3_665 ?
 O1W Mn1 O1W 82(2) 2_655 3_665 ?
 O9 Si1 O4 110.2(8) 5 . ?
 O9 Si1 O4 110.2(8) . . ?
 O9 Si1 O9 109.8(14) 5 . ?
 O9 Si1 O19 108.5(9) . . ?
 O9 Si1 O19 108.5(9) 5 . ?
 O19 Si1 O4 109.5(14) . . ?
 W1 Cs1 W5 56.05(4) 14_544 18_544 ?
 O10 Cs1 W1 25.6(4) 14_544 14_544 ?
 O10 Cs1 W5 79.7(4) 14_544 18_544 ?
 O10 Cs1 O11 51.1(5) 14_544 14_544 ?
 O10 Cs1 O13 48.4(5) 14_544 14_544 ?
 O10 Cs1 O13 128.8(5) 14_544 . ?
 O10 Cs1 O16 72.1(5) 14_544 . ?
 O10 Cs1 O18 89.9(5) 14_544 . ?
 O10 Cs1 O20 88.9(5) 14_544 14_544 ?
 O10 Cs1 O22 100.6(6) 14_544 18_544 ?
 O10 Cs1 O24 82.4(5) 14_544 18_544 ?
 O11 Cs1 W1 28.9(3) 14_544 14_544 ?
 O11 Cs1 W5 28.7(3) 14_544 18_544 ?
 O11 Cs1 O13 43.3(5) 14_544 14_544 ?
 O11 Cs1 O20 78.7(5) 14_544 14_544 ?
 O11 Cs1 O24 42.5(5) 14_544 18_544 ?
 O12 Cs1 W1 130.6(4) . 14_544 ?
 O12 Cs1 W5 165.9(4) . 18_544 ?
 O12 Cs1 O10 105.2(5) . 14_544 ?
 O12 Cs1 O11 152.4(5) . 14_544 ?
 O12 Cs1 O13 50.2(5) . . ?
 O12 Cs1 O13 135.5(5) . 14_544 ?
 O12 Cs1 O16 49.5(5) . . ?
 O12 Cs1 O18 83.7(5) . . ?
 O12 Cs1 O20 118.9(5) . 14_544 ?
 O12 Cs1 O22 141.8(6) . 18_544 ?
 O12 Cs1 O24 162.7(5) . 18_544 ?
 O13 Cs1 W1 30.2(3) 14_544 14_544 ?
 O13 Cs1 W1 143.9(4) . 14_544 ?
 O13 Cs1 W5 116.3(4) . 18_544 ?
 O13 Cs1 W5 57.5(3) 14_544 18_544 ?
 O13 Cs1 O11 129.2(5) . 14_544 ?
 O13 Cs1 O13 172.5(4) . 14_544 ?
 O13 Cs1 O16 58.1(5) . . ?
 O13 Cs1 O18 49.1(5) . . ?
 O13 Cs1 O20 43.8(5) 14_544 14_544 ?
 O13 Cs1 O20 141.3(5) . 14_544 ?
 O13 Cs1 O22 91.7(6) . 18_544 ?
 O13 Cs1 O24 41.0(5) 14_544 18_544 ?
 O13 Cs1 O24 135.7(5) . 18_544 ?
 O16 Cs1 W1 94.4(3) . 14_544 ?
 O16 Cs1 W5 122.4(3) . 18_544 ?
 O16 Cs1 O11 104.4(5) . 14_544 ?
 O16 Cs1 O13 120.3(5) . 14_544 ?
 O16 Cs1 O20 150.5(5) . 14_544 ?
 O16 Cs1 O24 146.9(4) . 18_544 ?
 O18 Cs1 W1 95.7(4) . 14_544 ?
 O18 Cs1 W5 83.0(4) . 18_544 ?
 O18 Cs1 O11 82.5(5) . 14_544 ?
 O18 Cs1 O13 123.8(5) . 14_544 ?
 O18 Cs1 O16 48.8(5) . . ?
 O18 Cs1 O20 156.7(5) . 14_544 ?
 O18 Cs1 O24 112.2(5) . 18_544 ?
 O20 Cs1 W1 74.0(3) 14_544 14_544 ?
 O20 Cs1 W5 73.9(3) 14_544 18_544 ?
 O22 Cs1 W1 79.6(4) 18_544 14_544 ?
 O22 Cs1 W5 25.5(4) 18_544 18_544 ?
 O22 Cs1 O11 50.8(5) 18_544 14_544 ?
 O22 Cs1 O13 82.6(5) 18_544 14_544 ?
 O22 Cs1 O16 116.2(5) 18_544 . ?
 O22 Cs1 O18 68.5(5) 18_544 . ?
 O22 Cs1 O20 88.9(5) 18_544 14_544 ?
 O22 Cs1 O24 47.6(5) 18_544 18_544 ?
 O24 Cs1 W1 57.2(3) 18_544 14_544 ?
 O24 Cs1 W5 29.2(3) 18_544 18_544 ?
 O24 Cs1 O20 44.7(4) 18_544 14_544 ?
 O2 Cs2 O2 48.2(6) 17_445 13_445 ?
 O2 Cs2 O2 48.2(6) 14_545 18_545 ?
 O2 Cs2 O2 116.0(2) 17_445 18_545 ?
 O2 Cs2 O2 116.0(2) 17_445 16 ?
 O2 Cs2 O2 116.0(2) 16 18_545 ?
 O2 Cs2 O2 48.2(6) 15 16 ?
 O2 Cs2 O2 69.1(6) 16 14_545 ?
 O2 Cs2 O2 154.3(7) 15 18_545 ?
 O2 Cs2 O2 154.3(7) 16 13_445 ?
 O2 Cs2 O2 116.0(2) 15 13_445 ?
 O2 Cs2 O2 116.0(2) 15 14_545 ?
 O2 Cs2 O2 69.1(6) 15 17_445 ?
 O2 Cs2 O2 154.3(7) 17_445 14_545 ?
 O2 Cs2 O2 116.0(2) 13_445 14_545 ?
 O2 Cs2 O2 69.1(6) 13_445 18_545 ?
 O2 Cs2 O5 52.0(5) 15 15 ?
 O2 Cs2 O5 90.7(3) 16 15 ?
 O2 Cs2 O5 90.7(3) 17_445 13_445 ?
 O2 Cs2 O5 90.7(3) 18_545 14_545 ?
 O2 Cs2 O5 152.0(4) 15 13_445 ?
 O2 Cs2 O5 152.0(4) 17_445 14_545 ?
 O2 Cs2 O5 152.0(4) 16 13_445 ?
 O2 Cs2 O5 52.0(5) 17_445 15 ?
 O2 Cs2 O5 90.7(3) 15 14_545 ?
 O2 Cs2 O5 52.0(5) 18_545 13_445 ?
 O2 Cs2 O5 52.0(5) 16 14_545 ?
 O2 Cs2 O5 90.7(3) 13_445 15 ?
 O2 Cs2 O5 52.0(5) 14_545 14_545 ?
 O2 Cs2 O5 152.0(4) 13_445 14_545 ?
 O2 Cs2 O5 52.0(5) 13_445 13_445 ?
 O2 Cs2 O5 152.0(4) 14_545 15 ?
 O2 Cs2 O5 90.7(3) 14_545 13_445 ?
 O2 Cs2 O5 152.0(4) 18_545 15 ?
 O5 Cs2 O5 100.4(7) 15 13_445 ?
 O5 Cs2 O5 100.4(7) 13_445 14_545 ?
 O5 Cs2 O5 100.4(7) 15 14_545 ?
 O6 Cs2 O2 100.4(3) 15 17_445 ?
 O6 Cs2 O2 47.9(5) 14_545 14_545 ?
 O6 Cs2 O2 47.9(5) 15 16 ?
 O6 Cs2 O2 142.5(4) 15 18_545 ?
 O6 Cs2 O2 47.9(5) 14_545 18_545 ?
 O6 Cs2 O2 100.4(3) 14_545 13_445 ?
 O6 Cs2 O2 142.5(4) 14_545 15 ?
 O6 Cs2 O2 142.5(4) 13_445 16 ?
 O6 Cs2 O2 100.4(3) 13_445 18_545 ?
 O6 Cs2 O2 47.9(5) 13_445 13_445 ?
 O6 Cs2 O2 100.4(3) 15 14_545 ?
 O6 Cs2 O2 142.5(4) 15 13_445 ?
 O6 Cs2 O2 100.4(3) 14_545 16 ?
 O6 Cs2 O2 47.9(5) 15 15 ?
 O6 Cs2 O2 47.9(5) 13_445 17_445 ?
 O6 Cs2 O2 142.5(4) 14_545 17_445 ?
 O6 Cs2 O2 100.4(3) 13_445 15 ?
 O6 Cs2 O2 142.5(4) 13_445 14_545 ?
 O6 Cs2 O5 52.1(2) 15 14_545 ?
 O6 Cs2 O5 52.1(2) 13_445 15 ?
 O6 Cs2 O5 52.1(2) 14_545 13_445 ?
 O6 Cs2 O5 122.7(7) 13_445 14_545 ?
 O6 Cs2 O5 52.10(19) 15 15 ?
 O6 Cs2 O5 52.1(2) 13_445 13_445 ?
 O6 Cs2 O5 122.7(7) 14_545 15 ?
 O6 Cs2 O5 52.1(2) 14_545 14_545 ?
 O6 Cs2 O5 122.7(7) 15 13_445 ?
 O6 Cs2 O6 97.3(6) 13_445 15 ?
 O6 Cs2 O6 97.3(6) 15 14_545 ?
 O6 Cs2 O6 97.3(6) 13_445 14_545 ?
 Nb2 Cs3 Nb1 52.20(7) 16_554 15_554 ?
 Nb2 Cs3 Nb1 90.87(8) 14_544 15_554 ?
 Nb2 Cs3 Nb2 54.65(9) 16_554 14_544 ?
 O2 Cs3 Nb1 26.5(4) 16_554 15_554 ?
 O2 Cs3 Nb1 86.4(3) 14_544 15_554 ?
 O2 Cs3 Nb2 25.8(4) 14_544 14_544 ?
 O2 Cs3 Nb2 70.0(4) 16_554 14_544 ?
 O2 Cs3 Nb2 25.8(4) 16_554 16_554 ?
 O2 Cs3 Nb2 70.0(4) 14_544 16_554 ?
 O2 Cs3 O2 74.8(7) 16_554 14_544 ?
 O2 Cs3 O3 115.7(5) 16_554 18_544 ?
 O2 Cs3 O3 115.7(5) 14_544 15_554 ?
 O2 Cs3 O3 51.2(5) 16_554 15_554 ?
 O2 Cs3 O3 51.2(5) 14_544 18_544 ?
 O2 Cs3 O7 50.5(5) 14_544 14_544 ?
 O2 Cs3 O7 50.5(5) 16_554 16_554 ?
 O2 Cs3 O7 91.8(5) 16_554 14_544 ?
 O2 Cs3 O7 91.8(5) 14_544 16_554 ?
 O2 Cs3 O11 57.5(5) 14_544 14_544 ?
 O2 Cs3 O11 129.2(5) 16_554 14_544 ?
 O2 Cs3 O11 57.5(5) 16_554 16_554 ?
 O2 Cs3 O11 129.2(5) 14_544 16_554 ?
 O3 Cs3 Nb1 109.2(3) 18_544 15_554 ?
 O3 Cs3 Nb1 30.2(3) 15_554 15_554 ?
 O3 Cs3 Nb2 120.3(4) 15_554 14_544 ?
 O3 Cs3 Nb2 72.8(4) 15_554 16_554 ?
 O3 Cs3 Nb2 72.8(4) 18_544 14_544 ?
 O3 Cs3 Nb2 120.3(4) 18_544 16_554 ?
 O3 Cs3 O3 121.4(7) 15_554 18_544 ?
 O3 Cs3 O11 166.4(5) 18_544 16_554 ?
 O3 Cs3 O11 45.0(5) 18_544 14_544 ?
 O3 Cs3 O11 166.4(5) 15_554 14_544 ?
 O3 Cs3 O11 45.0(5) 15_554 16_554 ?
 O7 Cs3 Nb1 116.8(4) 14_544 15_554 ?
 O7 Cs3 Nb1 72.5(3) 16_554 15_554 ?
 O7 Cs3 Nb2 69.0(3) 16_554 14_544 ?
 O7 Cs3 Nb2 69.0(3) 14_544 16_554 ?
 O7 Cs3 Nb2 30.3(3) 16_554 16_554 ?
 O7 Cs3 Nb2 30.3(3) 14_544 14_544 ?
 O7 Cs3 O3 80.0(5) 14_544 18_544 ?
 O7 Cs3 O3 141.8(5) 14_544 15_554 ?
 O7 Cs3 O3 141.8(5) 16_554 18_544 ?
 O7 Cs3 O3 80.0(5) 16_554 15_554 ?
 O7 Cs3 O7 66.7(7) 16_554 14_544 ?
 O7 Cs3 O11 45.4(5) 16_554 16_554 ?
 O7 Cs3 O11 110.8(5) 16_554 14_544 ?
 O7 Cs3 O11 110.8(5) 14_544 16_554 ?
 O7 Cs3 O11 45.4(5) 14_544 14_544 ?
 O11 Cs3 Nb1 143.4(3) 14_544 15_554 ?
 O11 Cs3 Nb1 59.0(3) 16_554 15_554 ?
 O11 Cs3 Nb2 112.2(3) 16_554 14_544 ?
 O11 Cs3 Nb2 59.6(3) 14_544 14_544 ?
 O11 Cs3 Nb2 112.2(3) 14_544 16_554 ?
 O11 Cs3 Nb2 59.6(3) 16_554 16_554 ?
 O11 Cs3 O11 148.6(6) 16_554 14_544 ?
 O17 Cs3 Nb1 135.89(13) . 15_554 ?
 O17 Cs3 Nb2 105.4(6) . 14_544 ?
 O17 Cs3 Nb2 105.4(6) . 16_554 ?
 O17 Cs3 O2 124.6(6) . 16_554 ?
 O17 Cs3 O2 124.6(6) . 14_544 ?
 O17 Cs3 O3 114.7(4) . 18_544 ?
 O17 Cs3 O3 114.7(4) . 15_554 ?
 O17 Cs3 O7 75.7(6) . 14_544 ?
 O17 Cs3 O7 75.7(6) . 16_554 ?
 O17 Cs3 O11 76.9(3) . 14_544 ?
 O17 Cs3 O11 76.9(3) . 16_554 ?
 O2W Na1 O17 65.1(13) . 15 ?
 Nb1 O1 Mn1 175.3(17) . . ?
 Nb1 O1 Cs2 89.9(10) . 7_554 ?
 Mn1 O1 Cs2 94.8(9) . 7_554 ?
 Nb1 O2 Cs2 88.8(7) . 7_554 ?
 Nb1 O2 Cs3 107.1(8) . 9 ?
 Nb2 O2 Nb1 144.2(11) . . ?
 Nb2 O2 Cs2 90.4(7) . 7_554 ?
 Nb2 O2 Cs3 107.7(8) . 9 ?
 Cs3 O2 Cs2 104.8(5) 9 7_554 ?
 W5 O3 Nb1 119.7(10) . . ?
 W5 O3 Cs3 113.4(8) . 8 ?
 Nb1 O3 Cs3 94.5(7) . 8 ?
 W5 O4 W5 91.1(8) 5 . ?
 W5 O4 Nb1 92.7(7) 5 . ?
 W5 O4 Nb1 92.7(7) . . ?
 Si1 O4 W5 124.6(7) . . ?
 Si1 O4 W5 124.6(7) . 5 ?
 Si1 O4 Nb1 121.9(12) . . ?
 Nb2 O5 Nb2 153.2(18) 6_655 . ?
 Nb2 O5 Cs2 89.2(9) 6_655 7_554 ?
 Nb2 O5 Cs2 89.2(9) . 7_554 ?
 Nb2 O6 Nb2 141.6(15) 5 . ?
 Nb2 O6 Cs2 93.2(8) 5 7_554 ?
 Nb2 O6 Cs2 93.2(8) . 7_554 ?
 W1 O7 Nb2 118.8(10) . . ?
 W1 O7 Cs3 114.9(9) . 9 ?
 Nb2 O7 Cs3 96.7(7) . 9 ?
 W2 O8 Nb2 118.5(10) . . ?
 W1 O9 Nb2 90.3(6) . . ?
 W2 O9 W1 91.6(6) . . ?
 W2 O9 Nb2 90.1(6) . . ?
 Si1 O9 W1 125.6(10) . . ?
 Si1 O9 W2 126.5(10) . . ?
 Si1 O9 Nb2 122.1(10) . . ?
 W1 O10 Cs1 104.0(9) . 9 ?
 W1 O11 Cs1 93.2(7) . 9 ?
 W1 O11 Cs3 99.0(7) . 9 ?
 W5 O11 W1 153.4(11) 5 . ?
 W5 O11 Cs1 93.8(7) 5 9 ?
 W5 O11 Cs3 102.9(7) 5 9 ?
 Cs1 O11 Cs3 108.6(5) 9 9 ?
 W1 O12 W2 118.2(10) . . ?
 W1 O12 Cs1 107.7(8) . . ?
 W2 O12 Cs1 108.5(7) . . ?
 W1 O13 Cs1 102.4(8) . . ?
 W1 O13 Cs1 84.1(6) . 9 ?
 W4 O13 W1 150.0(12) . . ?
 W4 O13 Cs1 105.7(8) . . ?
 W4 O13 Cs1 95.8(8) . 9 ?
 Cs1 O13 Cs1 110.4(6) . 9 ?
 W2 O15 W2 150.1(17) 5 . ?
 W2 O16 Cs1 102.1(7) . . ?
 W3 O16 W2 151.1(11) . . ?
 W3 O16 Cs1 105.6(7) . . ?
 W3 O17 Cs3 123.8(15) . . ?
 W3 O17 Na1 105.5(13) . 8_554 ?
 Na1 O17 Cs3 130.7(11) 8_554 . ?
 W3 O18 Cs1 103.5(8) . . ?
 W4 O18 W3 119.3(10) . . ?
 W4 O18 Cs1 102.3(8) . . ?
 W3 O19 W4 92.6(8) . . ?
 W3 O19 W4 92.6(8) . 5 ?
 W4 O19 W4 92.2(10) 5 . ?
 Si1 O19 W3 123.9(16) . . ?
 Si1 O19 W4 123.3(9) . 5 ?
 Si1 O19 W4 123.3(9) . . ?
 W4 O20 Cs1 94.8(8) . 9 ?
 W4 O21 W4 123.1(16) 5 . ?
 W5 O22 Cs1 100.2(9) . 12 ?
 W5 O23 W5 119.8(15) 5 . ?
 W4 O24 W5 151.9(12) 5 . ?
 W4 O24 Cs1 93.0(7) 5 12 ?
 W5 O24 Cs1 82.9(6) . 12 ?
 O5W O2W Na1 132(3) 7_455 . ?
 O3W O5W O2W 177(6) 9_554 13_544 ?

_shelx_SHELXL_version_number      '2014/7'
_olex2_submission_special_instructions 'No special instructions were received'
loop_
  _twin_individual_id
  _twin_individual_mass_fraction_refined
 1 0.331(18)
 2 0.669(18)

